LMucko/crystallography-open-database huggingface dataset:
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501529
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.89455(9)
_cell_length_b                   2.89455(9)
_cell_length_c                   2.83211(12)
_cell_volume                     20.5496(13)
_diffrn_ambient_pressure         4530000
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC58.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501529
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501530
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.88442(9)
_cell_length_b                   2.88442(9)
_cell_length_c                   2.82371(12)
_cell_volume                     20.3455(12)
_diffrn_ambient_pressure         8785000
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC59.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501530
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501531
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.87567(9)
_cell_length_b                   2.87567(9)
_cell_length_c                   2.81714(12)
_cell_volume                     20.1752(12)
_diffrn_ambient_pressure         12425000
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC60.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501531
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501532
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.85839(9)
_cell_length_b                   2.85839(9)
_cell_length_c                   2.80429(12)
_cell_volume                     19.8425(12)
_diffrn_ambient_pressure         20177500
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC61.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501532
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501533
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.85075(9)
_cell_length_b                   2.85075(9)
_cell_length_c                   2.79941(12)
_cell_volume                     19.7022(12)
_diffrn_ambient_pressure         23360000
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC62.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501533
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501534
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.84482(9)
_cell_length_b                   2.84482(9)
_cell_length_c                   2.79406(12)
_cell_volume                     19.5829(12)
_diffrn_ambient_pressure         26550000
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC63.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501534
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501535
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.83614(13)
_cell_length_b                   2.83614(13)
_cell_length_c                   2.78648(13)
_cell_volume                     19.4107(16)
_diffrn_ambient_pressure         30870000
_diffrn_ambient_temperature      473
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC64.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501535
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501536
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.89570(9)
_cell_length_b                   2.89570(9)
_cell_length_c                   2.83321(13)
_cell_volume                     20.5739(13)
_diffrn_ambient_pressure         5057500
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC65.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501536
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501537
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.88609(9)
_cell_length_b                   2.88609(9)
_cell_length_c                   2.82417(12)
_cell_volume                     20.3724(12)
_diffrn_ambient_pressure         9630000
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC66.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501537
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501538
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.87688(9)
_cell_length_b                   2.87688(9)
_cell_length_c                   2.81777(14)
_cell_volume                     20.1967(13)
_diffrn_ambient_pressure         13045000
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC67.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501538
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501539
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.85980(9)
_cell_length_b                   2.85980(9)
_cell_length_c                   2.80550(12)
_cell_volume                     19.8707(12)
_diffrn_ambient_pressure         20522500
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC68.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501539
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501540
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.85203(9)
_cell_length_b                   2.85203(9)
_cell_length_c                   2.80076(12)
_cell_volume                     19.7294(12)
_diffrn_ambient_pressure         23685000
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC69.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501540
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501541
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.84648(9)
_cell_length_b                   2.84648(9)
_cell_length_c                   2.79542(12)
_cell_volume                     19.6153(12)
_diffrn_ambient_pressure         26680000
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC70.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501541
Pressure-volume-temperature equation of state of tungsten carbide to 32 GPa and 1673 K
Litasov, Konstantin D.; Shatskiy, Anton; Fei, Yingwei; Suzuki, Akio; Ohtani, Eiji; Funakoshi, Kenichi; Journal of Applied Physics 108 (2010) –; doi:10.1063/1.3481667

data_1501542
_publ_section_title
;
 Pressure-volume-temperature equation of state of tungsten carbide to 32
 GPa and 1673 K
;
_journal_issue                   5
_journal_name_full               'Journal of Applied Physics'
_journal_paper_doi               10.1063/1.3481667
_journal_volume                  108
_journal_year                    2010
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.83895(9)
_cell_length_b                   2.83895(9)
_cell_length_c                   2.78842(18)
_cell_volume                     19.4628(15)
_diffrn_ambient_pressure         30832500
_diffrn_ambient_temperature      673
_journal_article_reference       053513
_cod_data_source_file            WC_P-6m2_DC71.cif
_cod_data_source_block           chateigner_
_cod_original_formula_sum        'W C'
_cod_database_code               1501542
Supramolecular Chromotropism of the Crystalline Phases of 4,5,6,7-Tetrafluorobenzo-2,1,3-telluradiazole
Anthony F. Cozzolino; Pamela S. Whitfield; Ignacio Vargas-Baca; Journal of the American Chemical Society 132 (2010) 17265–17270; doi:10.1021/ja107252f

data_4103653
_publ_contact_author_address
;Department of Chemistry
McMaster University
1280 Main St. W.
Hamilton, ON
L8S4M1
;
_publ_contact_author_email       vargas@chemistry.mcmaster.ca
_publ_contact_author_fax         1(905)5222509
_publ_contact_author_name        'Professor Ignacio Vargas-Baca'
_publ_contact_author_phone       1(905)5259140x23497
_publ_section_title
;
 Supramolecular Chromotropism of the Crystalline Phases of
 4,5,6,7-Tetrafluorobenzo-2,1,3-telluradiazole
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              17265
_journal_page_last               17270
_journal_paper_doi               10.1021/ja107252f
_journal_volume                  132
_journal_year                    2010
_chemical_formula_moiety         'C6 F4 N2 Te'
_chemical_formula_sum            'C6 F4 N2 Te'
_chemical_formula_weight         303.68
_chemical_name_common            4,5,6,7-tetrafluorobenzo-2,1,3-telluradiazole
_chemical_name_systematic        4,5,6,7-tetrafluorobenzo-2,1,3-telluradiazole
_chemical_properties_physical
'air-sensitive, moisture-sensitive, thermochromic'
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.2089(78)
_cell_angle_beta                 89.8747(62)
_cell_angle_gamma                90.0009(22)
_cell_formula_units_Z            2
_cell_length_a                   3.966833(86)
_cell_length_b                   11.54303(61)
_cell_length_c                   7.99022(40)
_cell_volume                     365.86(3)
_diffrn_ambient_pressure         101.3
_diffrn_ambient_temperature      84
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.540560
_exptl_crystal_colour            yellow
_exptl_crystal_description       powder
_exptl_crystal_recrystallization_method 'dynamic vacuum sublimation'
_cod_data_source_file            ja107252f_si_003.cif
_cod_data_source_block           beta6
_cod_original_cell_volume        365.863(33)
_cod_database_code               4103653